Shaped, Flat, Square, Round, Fine Wire, Plated and Un-plated
Type 316Ti is a titanium stabilized variation of alloy 316. This austenitic chromium-nickel stainless steel containing molybdenum which increases the corrosion resistance, improves resistance to pitting chloride ion solutions and provide increased strength at elevated temperatures. Properties are similar to those of alloy 316 except that 316Ti due to its Titanium addition can be used at elevated sensitization temperatures. Corrosion resistance is improved, particularly against sulfuric, hydrochloric, acetic, formic and tartaric acids, acid sulfates and alkaline chlorides.
Screening application in marine environment
Pulp and Paper Equipment
Propeller shafts, Fittings
Exterior Architectural components in Marine Coastal Areas
Carbon: 0.08 max
Manganese: 2.00 max
Silicon: 1.00 max
Titanium: 5 x (Carbon + Nitrogen) – 0.07
Phosphorus: 0.040 max
Sulfur: 0.030 max
Copper: 0.075 max
Density: 0.29 lbs/in³, 7.99 g/cm³
Electrical Resistivity: microhm-in (microhm-cm):
68°F (20°C): 29.4 (74.0)
Specific Heat: BTU/lb/°F (kJ/kg•K):
32-212°F (0-100°C): 0.12 (0.50)
Thermal Conductivity: BTU/hr/ft²/ft/°F (W/m•K):
At 212°F (100°C): 9.4 (16.2)
At 932°F (500°C): 12.4 (21.4)
Mean Coefficient of Thermal Expansion, in/in/°F (μm/m•K):
32-212°F (0-100°C): 8.9 x 10-6(16.0)
32-600°F (0-315°C): 9.0 x 10-6(16.2)
32-1000°F (0-538°C): 9.7 x 10-6 (17.5)
32-1200°F (0-649°C): 10.3 x 10-6 (18.5)
32-1500ºF (0-871ºC): 11.1 x 10-6 (18.5)
Modulus of Elasticity: KSI (MPa)
28.0 x 10³(193 x 10³) in tension
11.2 x 10³(77 x 10³) in torsion
Magnetic Permeability: H = 200 Oersteds: Annealed: < 1.02 max.
Melting Range: °F (°C) 2500 – 2590 (1371 – 1421)
Mechanical Properties at Room Temperature
Ultimate Tensile Strength: 75 KSI min (515 MPa min)
Yield Strength: (0.2% Offset) 30 KSI min (205 MPa min)
Elongation: 40% min
Hardness: Rb 95 max
Ultimate Tensile Strength: 85 KSI min (585 MPa min)
Yield Strength: (0.2% Offset) 45 KSI min (310 MPa min)
Elongation: 35% min
Ultimate Tensile Strength: 100 KSI min (690 MPa min)
Yield Strength: (0.2% Offset) 55 KSI min (380 MPa min)
Elongation: 35% min
Ultimate Tensile Strength: 125 KSI min (860 MPa min)
Yield Strength: (0.2% Offset) 75 KSI min (515 MPA min)
Elongation: 10% min
Alloy 316Ti can be cold rolled to achieve the temper properties required by specific customers and/or manufacturing requirements. Contact Ulbrich Wire for details.
See NACE (National Association of Corrosion Engineers) for more information.
Alloy 316Ti can be readily formed and drawn.
Standard Wire Finishes
Extra Clean: (XC) Extra clean is also referred to as “bright annealed” or “bright annealed and cold rolled”
Grease (round wire only): Drawn in a heavy grease produces an “Ultra bright” finish for decorative applications
Soap (round wire only): Soap is used as a lubricant in the drawing process and is not removed. It acts as a lubricant during customer part forming operation. A soap finish is available in tempered products.
Plated: Many plating options are available.
∗Special finishes are available: Contact Ulbrich Wire Sales with special finish and plating requests.
Cut to lengths
Alloy 316Ti is non hardenable by heat treatment.
For best results refer to: SSINA’s “Welding of Stainless Steels and Other Joining Methods”.
Limitation of Liability and Disclaimer of Warranty: In no event will Ulbrich Stainless Steels and Special Metals, Inc., be liable for any damages arising from the use of the information included in this document or that it is suitable for the ‘applications’ noted. We believe the information and data provided to be accurate to the best of our knowledge but, all data is considered typical values only. It is intended for reference and general information and not recommended for specification, design or engineering purposes. Ulbrich assumes no implied or express warranty in regard to the creation or accuracy of the data provided in this document.
Copyright© January 2014 Ulbrich Stainless Steels & Special Metals, Inc. – Revision 6.1.2015